HAL Id: hal-01528359
Submitted on 29 May 2017
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Increase in Capacitance by Subnanometer Pores in
Nicolas Jäckel, Patrice Simon, Yury Gogotsi, Volker Presser
To cite this version:
Nicolas Jäckel, Patrice Simon, Yury Gogotsi, Volker Presser. Increase in Capacitance by
Subnanome-ter Pores in Carbon. ACS Energy LetSubnanome-ters, American Chemical Society 2016, 1 (6), pp.1262-1265.
OATAO is an open access repository that collects the work of Toulouse researchers and
makes it freely available over the web where possible.
This is an author-deposited version published in :
Eprints ID : 16683
To link to this article :
URL : http://dx.doi.org/10.1021/acsenergylett.6b00516
To cite this version :
Jäckel, Nicolas and Simon, Patrice and
Gogotsi, Yury and Presser, Volker Increase in Capacitance by
Subnanometer Pores in Carbon. (2016) ACS Energy Letters, vol. 1
(n° 6). pp. 1262-1265. ISSN 2380-8195
Any correspondence concerning this service should be sent to the repository
Increase in Capacitance by Subnanometer
Pores in Carbon
Electrical double-layer capacitors (EDLCs, also known as supercapacitors or ultracapacitors) store energy by electrosorption of ions at the electrode/electrolyte interface.1To achieve a high-energy storage capacity, electrodes with a high surface area and well-developed pore structure in the range from several Angstroms to several tens of nanometers are required.2 However, neither natural precursor-derived carbons nor templated carbon materials present an ideal, inﬁnitesimally narrow pore size dispersion.3
In EDLCs, the use of salt dissolved in an organic or aqueous solvent makes it important to consider the solvation shell around the ions. The bare ion size is usually below 1 nm, whereas the solvation shell can increase the size signiﬁcantly.3 Several studies have provided strong evidence of ion desolva-tion during electrosorpdesolva-tion, which is the only way to explain why carbon materials with pore sizes smaller than the solvated ion but larger than the bare ion have high charge storage capacities.4−8 A maximized capacitance (normalized by the
surface area) was found in experimental and theoretical studies when matching the pore size with the ion size.9 This eﬀect seems to be universally applicable for solvent-containing and solvent-free electrolytes (ionic liquids), while important secondary diﬀerences are to be considered for the latter. For example, the oscillatory dependency of capacitance on pore size predicted for neat ionic liquids and ideal carbons with slit pores is lost when introducing a solvent, where a single maximum is observed when the ion size and the pore size are identical.10,11 This Viewpoint clariﬁes the correlation between capacitance and pore size, which is of high practical importance for the design of advanced carbon electrode materials. Two extreme cases are obvious: excessively large pores, accompanied by large pore volumes and limited speciﬁc surface area, will lead to a low energy storage capacity, whereas very small pores will limit the ion access due to steric eﬀects (Figure 1), in addition to imposing obstacles to ion transport.12,13 Yet, for the
intermediate range, down to the point when the pores are too small for the bare ion to ﬁt, there is no consent in the literature about the correlation between the pore size and the corresponding area-normalized capacitance. For example, there has been criticism about the method of surface area determination and normalization, especially considering the inadequacy of the Brunauer−Emmett−Teller (BET) model for microporous carbons.14,15 Benchmarking various kinds of carbons, including carbon monoliths, a “regular pattern” was presented, suggesting that the area-normalized capacitance does not depend on the pore size.14,16This lack of dependence can
be explained by neither the ab initio or molecular dynamics models17,18 nor geometric considerations as when the pore
diameter increases by 50−90%, there is still just one ion in each pore contributing to charge storage and the remaining surface area and pore volume remain unused, decreasing the capacitance normalized by the pore surface or volume.
Recently, we developed a model for understanding the capacitance of microporous carbons, taking into account the entire measured pore size distribution, and have established a comprehensive data set of electrochemical measurements.6 Density functional theory (DFT) kernels were used, which are currently the most advanced methodology to extract porosity data from gas sorption isotherms for meso- and microporous carbons and eﬀectively avoid the fundamental limitations of the BET theory.19 Activated carbon showed the highest speciﬁc
surface area (SSA), followed by two diﬀerent titanium carbide-derived carbons (CDCs),20 activated carbon black (CB), and carbon onions.21 Yet, when normalizing electrochemical performance data on porosity values, we ﬁrst have to consider diﬀerences between dry powder and ﬁlm electrodes.6Then, we have to assess the diﬀerences in pore size distributions; these are shown in Figure 2A normalized to 100% for the aforementioned carbon materials. Many carbons display a signiﬁcant dispersion width; this is why the often-used volume-weighted average pore size d50does not fully capture the pore
size distribution width, as we show by adding values for d25and
d75, representing the pore width encompassing 25 and 75% of
the total pore volume, respectively (Table 1,Figure 2A). More diﬀerences in the surface area of the diﬀerent electrode materials become evident when we calculate the electrochemi-cally active surface, that is, the ion-accessible surface area (Table 1,Figure 2B). Taking into account the bare ion size of BF4−(0.45 nm) and TEA+(0.67 nm), pores smaller than these
Figure 1. Electrosorption of speciﬁc ions with a ﬁnite size is only possible if the pore size is at least equal to the ion size. Therefore, the speciﬁc surface area of pores smaller than the bare ion size is inaccessible for energy storage. Larger pores can adsorb more than one ion per pore.
values are inaccessible to the ions.7 The result is a further reduction of the speciﬁc surface area, and we have to consider diﬀerent cutoﬀ values for the positively (cutoﬀ pore size of 0.4 nm) and negatively (cutoﬀ at 0.6 nm) polarized electrodes. In
the case of CDC, only about 40−50% of the total SSA is accessible to TEA+compared to about 70% for activated carbon
and carbon black (Figure 2A).
The reported electrochemical measurements using a three-electrode conﬁguration (for experimental methods see the
Supporting Information) showed a nonlinear correlation of SSA and gravimetric capacitance measured in F·g−1(Table 1)
for 1 M TEA-BF4in acetonitrile (ACN) or propylene carbonate
(PC).6 A very high Coulombic eﬃciency (up to 99%) underlines the absence of signiﬁcant Faradaic reactions in the chosen potential window (Table 1). When we normalize the measured electrode capacitance by the surface area accessible to cations or anions at +1 and −1 V vs carbon, respectively, we see a clear diﬀerence between positive and negative polarization (Figure 3, Table 1). Instead of just discussing the electro-chemical data in the context of average pore width (d50), we
added error bars for the x-axis, which spread between d25 and
d75(Figure 3). Even when considering pore size dispersity, we
still see a clear trend of increased normalized capacitance in subnanometer pores, which is signiﬁcantly larger for negative polarization (i.e., electrosorption of the larger TEA+ cation).
The more eﬀective use of available pores in the case of matching sizes results in a strong increase in capacitance, which was already shown by a geometric model of Huang et al. (ref
22; see also the data line inFigure 3). For larger pore sizes, in
Figure 2. (A) The cumulative pore size distribution of electrodes was derived by combining CO2and N2sorption and normalizing all data to
100%. (B) Porosity analysis of diﬀerent carbon electrode materials using a DFT model. Data are normalized for SSA of electrodes containing 10 mass% PTFE as 100% and the calculated accessible surface area for BF4−anions (0.4 nm, BF4−accessible) and TEA+cations (0.6 nm, TEA+
Table 1. Combined NLDFT Model for CO2Sorption for Pores Smaller than 0.9 nm and QSDFT Model for N2Sorption for
Pores Larger than 0.9 nma
Material DFT SSA (m2· g−1) d50(dwidth (nm)25−d75) pore capacitance at +1 V in ACN (F·g−1) Coulomb eﬃciency (%) capacitance at +1 V in PC (F·g−1) Coulomb eﬃciency (%) capacitance at −1 V in ACN (F·g−1) Coulomb eﬃciency (%) capacitance at −1 V in PC (F·g−1) Coulomb eﬃciency (%) AC 1839 1.3 (0.8−1.8) 113 96 115 99 103 99 102 99 CB 1097 15 (5−19) 99 99 99 99 88 99 87 99 OLC 232 9.5 (6−14) 20 98 20 99 16 99 16 99 CDC600 934 0.64 (0.53−0.93) 127 97 132 98 121 98 119 99 CDC1000 967 0.90 (0.62−1.4) 101 97 100 98 98 98 96 99 a
The average pore size relates to the volume-weighted arithmetic mean value d50with the standard deviation from d25to d75. Capacitance values were
recorded at +1 V vs carbon and −1 V vs carbon in a three-electrode setup (half-cell).
Figure 3. Capacitance of porous carbons normalized to the accessible surface area for each ion in both solvents. The regular pattern average of 0.95 F m−2from ref15is added, and data for the
particular, for mesopores, the capacitance converges toward an average value below 0.1 F·m−2, which aligns well with the “regular pattern” value reported by Centeno et al. (ref15) and with the calculated value limiting the double-layer capacitance at the planar carbon interface (or larger than the few-nm pores; ref17).
For electrolytes with signiﬁcant diﬀerences between the size of anions and cations, our data clearly show the importance of diﬀerentiating between ion electrosorption during positive or negative polarization with use of half-cell measurements (Figure 3). With a larger size of TEA+, and smaller corresponding
surface area accessible to the cations, the values of areal capacitance during negative polarization are signiﬁcantly larger than those for BF4−electrosorption (i.e., positive polarization).
Accordingly, advanced EDLC cell design could achieve performance enhancement by developing nanoporous carbon with slightly diﬀerent pore sizes for the positive and negative electrodes.23,24
In summary, our data analysis clearly supports the increase in surface-normalized capacitance when most of the pores are below 1 nm, in agreement with previous studies (e.g., see refs7
and25). This was shown for carbons with very diﬀerent pore structures considering the complexity of pore size dispersity and for two diﬀerent solvents (i.e., PC and ACN). This eﬀect is seen at diﬀerent amplitudes for positive and negative polarization, with a smaller increase for BF4−within the range
of investigated pore sizes.
INM - Leibniz Institute for New Materials, 66123 Saarbrücken, Germany
Department of Materials Science and Engineering, Saarland University, 66123 Saarbrücken, Germany
Université Paul Sabatier, CIRIMAT UMR, CNRS 5085, 5085, 31062 Toulouse Cedex 4, France
Réseau sur le Stockage Electrochimique de l′Energie, RS2E FR CNRS 3459, 80039 Amiens Cedex, France
⊥Department of Materials Science and Engineering, and A. J.
Drexel Nanotechnology Institute, Drexel University, Philadelphia, Pennsylvania 19104, United States
The authors thank Dr. Weingarth, Dr. Aslan, Anna Schreiber, Jeon Jeongwook (all at INM), and Katherine Van Aken (Drexel University) for their technical support and helpful discussion. N.J. and V.P. also thank Prof. Eduard Arzt (INM) for his continuing support. Y.G. was supported by the Fluid Interface Reactions, Structures and Transport (FIRST) Center, an Energy Frontier Research Center funded by the U.S. Department of Energy, Oﬃce of Science, Oﬃce of Basic Energy Sciences.
(1) Beguin, F.; Frackowiak, E. Supercapacitors; Wiley: Weinheim, Germany, 2013.
(2) Salanne, M.; Rotenberg, B.; Naoi, K.; Kaneko, K.; Taberna, P. L.; Grey, C. P.; Dunn, B.; Simon, P. Efficient storage mechanisms for building better supercapacitors. Nature Energy 2016, 1, 16070.
(3) Kondrat, S.; Perez, C. R.; Presser, V.; Gogotsi, Y.; Kornyshev, A. A. Effect of pore size and its dispersity on the energy storage in nanoporous supercapacitors. Energy Environ. Sci. 2012, 5, 6474−6479. (4) Kastening, B.; Spinzig, S. Electrochemical polarization of activated carbon and graphite powder suspensions: Part II. Exchange of ions between electrolyte and pores. J. Electroanal. Chem. Interfacial Electrochem. 1986, 214, 295−302.
(5) Levi, M. D.; Sigalov, S.; Salitra, G.; Aurbach, D.; Maier, J. The effect of specific adsorption of cations and their size on the charge-compensation mechanism in carbon micropores: The role of anion desorption. ChemPhysChem 2011, 12, 854−862.
(6) Jäckel, N.; Rodner, M.; Schreiber, A.; Jeongwook, J.; Zeiger, M.; Aslan, M.; Weingarth, D.; Presser, V. Anomalous or regular capacitance? The influence of pore size dispersity on double-layer formation. J. Power Sources 2016, 326, 660−671.
(7) Chmiola, J.; Yushin, G.; Gogotsi, Y.; Portet, C.; Simon, P.; Taberna, P. L. Anomalous increase in carbon capacitance at pore sizes less than 1 nm. Science 2006, 313, 1760−1763.
(8) Raymundo-Pinero, E.; Kierzek, K.; Machnikowski, J.; Beguin, F. Relationship between the nanoporous texture of activated carbons and their capacitance properties in different electrolytes. Carbon 2006, 44, 2498−2507.
(9) Largeot, C.; Portet, C.; Chmiola, J.; Taberna, P.-L.; Gogotsi, Y.; Simon, P. Relation between the ion size and pore size for an electric double-layer capacitor. J. Am. Chem. Soc. 2008, 130, 2730−2731.
(10) Jiang, D.; Jin, Z.; Henderson, D.; Wu, J. Solvent effect on the pore-size dependence of an organic electrolyte supercapacitor. J. Phys. Chem. Lett. 2012, 3, 1727−1731.
(11) Feng, G.; Qiao, R.; Huang, J.; Sumpter, B. G.; Meunier, V. Ion distribution in electrified micropores and its role in the anomalous enhancement of capacitance. ACS Nano 2010, 4, 2382−2390.
(12) Segalini, J.; Iwama, E.; Taberna, P.-L.; Gogotsi, Y.; Simon, P. Steric effects in adsorption of ions from mixed electrolytes into microporous carbon. Electrochem. Commun. 2012, 15, 63−65.
(13) Levi, M. D.; Levy, N.; Sigalov, S.; Salitra, G.; Aurbach, D.; Maier, J. Electrochemical quartz crystal microbalance (EQCM) studies of ions and solvents insertion into highly porous activated carbons. J. Am. Chem. Soc. 2010, 132, 13220−13222.
(14) Thommes, M.; Kaneko, K.; Neimark, A. V.; Olivier, J. P.; Rodriguez-Reinoso, F.; Rouquerol, J.; Sing, K. S. W. Physisorption of gases, with special reference to the evaluation of surface area and pore size distribution. Pure Appl. Chem. 2015, 87, 1051−1069.
(15) Centeno, T. A.; Sereda, O.; Stoeckli, F. Capacitance in carbon pores of 0.7 to 15 nm: a regular pattern. Phys. Chem. Chem. Phys. 2011, 13, 12403−6.
(16) Garcia-Gomez, A.; Moreno-Fernandez, G.; Lobato, B.; Centeno, T. A. Constant capacitance in nanopores of carbon monoliths. Phys. Chem. Chem. Phys. 2015, 17, 15687−90.
(17) Huang, J.; Sumpter, B. G.; Meunier, V.; Yushin, G.; Portet, C.; Gogotsi, Y. Curvature effects in carbon nanomaterials: Exohedral versus endohedral supercapacitors. J. Mater. Res. 2010, 25, 1525−1531. (18) Merlet, C.; Rotenberg, B.; Madden, P. A.; Taberna, P. L.; Simon, P.; Gogotsi, Y.; Salanne, M. On the molecular origin of super-capacitance in nanoporous carbon electrodes. Nat. Mater. 2012, 11, 306−10.
(19) Gor, G. Y.; Thommes, M.; Cychosz, K. A.; Neimark, A. V. Quenched solid density functional theory method for characterization of mesoporous carbons by nitrogen adsorption. Carbon 2012, 50, 1583−1590.
(20) Presser, V.; Heon, M.; Gogotsi, Y. Carbide-derived carbons − from porous networks to nanotubes and graphene. Adv. Funct. Mater. 2011, 21, 810−833.
(21) Zeiger, M.; Jäckel, N.; Aslan, M.; Weingarth, D.; Presser, V. Understanding structure and porosity of nanodiamond-derived carbon onions. Carbon 2015, 84, 584−598.
(22) Huang, J.; Sumpter, B. G.; Meunier, V. A universal model for nanoporous carbon supercapacitors applicable to diverse pore regimes, carbon materials, and electrolytes. Chem. - Eur. J. 2008, 14, 6614− 6626.
(23) Sigalov, S.; Levi, M. D.; Salitra, G.; Aurbach, D.; Jänes, A.; Lust, E.; Halalay, I. C. Selective adsorption of multivalent ions into TiC-derived nanoporous carbon. Carbon 2012, 50, 3957−3960.
(24) Weingarth, D.; Zeiger, M.; Jäckel, N.; Aslan, M.; Feng, G.; Presser, V. Graphitization as a universal tool to tailor the potential-dependent capacitance of carbon supercapacitors. Adv. Energy Mater. 2014, 4, 1400316.
(25) Chmiola, J.; Largeot, C.; Taberna, P.-L.; Simon, P.; Gogotsi, Y. Desolvation of Ions in subnanometer pores and its effect on capacitance and double-layer theory. Angew. Chem., Int. Ed. 2008, 47, 3392−3395.
(C2(:$%''%$8797>( ! " ! ./0*1*23'4('5*.(6&'&"&3*+$%*/37*0-&3%'-869*::;<=*!--%4%>?@3(9*A3%,-(B* < * C3#-%&,3(&*$+*0-&3%'-86*!?'3(?3*-(D*E()'(33%'()9*!--%8-(D*F('G3%6'&B9*::;<=*!--%4%>?@3(9*A3%,-(B* = * F('G3%6'&H*I-"8*!-4-&'3%9*J.K.0LM*F0K9*J/K!*NOPN9*NOPN9*=;O:<*M$"8$"63*J3D3Q*R9*S%-(?3* R* KH63-"*6"%*83*!&$?@-)3*E83?&%$?T','U"3*D3*8VE(3%)'39*K!<E*SK*J/K!*=RNW9*S%-(?3* N
* C3#-%&,3(&* $+* 0-&3%'-86* !?'3(?3* -(D* E()'(33%'()* X* LY* ZY* C%3Q38* /-($&3?T($8$)B* .(6&'&"&39* IL* ;W;OR* IT'8-D38#T'-9*F!L* *